Synthesis, crystal structure, magnetic and electronic properties of the caesium-based transition metal halide Cs3Fe2Br9
Wei, Fengxia; Brivio, Federico; Wu, Yue; Sun, Shijing; Bristowe, Paul D.; Cheetham, Anthony K.; Journal of Materials Chemistry C 6 (2018) 3573–; doi:10.1039/C7TC04798C

data_7236991
_publ_section_title
;
 Synthesis, crystal structure, magnetic and electronic properties of the
 caesium-based transition metal halide Cs3Fe2Br9
;
_journal_issue                   14
_journal_name_full               'Journal of Materials Chemistry C'
_journal_page_first              3573
_journal_paper_doi               10.1039/C7TC04798C
_journal_volume                  6
_journal_year                    2018
_chemical_formula_moiety         'Br9 Cs3 Fe2'
_chemical_formula_sum            'Br9 Cs3 Fe2'
_chemical_formula_weight         1229.62
_space_group_crystal_system      hexagonal
_space_group_IT_number           194
_space_group_name_Hall           '-P 6c 2c'
_space_group_name_H-M_alt        'P 63/m m c'
_atom_sites_solution_primary     direct
_audit_creation_date             2017-05-24
_audit_creation_method
;
Olex2 1.2
(compiled 2017.03.28 svn.r3405 for OlexSys, GUI svn.r5337)
;
_audit_update_record
;
2017-09-16 deposited with the CCDC.
2017-11-13 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   7.5427(8)
_cell_length_b                   7.5427(8)
_cell_length_c                   18.5849(13)
_cell_measurement_reflns_used    772
_cell_measurement_temperature    298.6(3)
_cell_measurement_theta_max      27.6080
_cell_measurement_theta_min      2.1760
_cell_volume                     915.68(15)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.34i (release 04-08-2014 CrysAlis171 .NET)
(compiled Aug  4 2014,14:34:23)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.34i (release 04-08-2014 CrysAlis171 .NET)
(compiled Aug  4 2014,14:34:23)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.34i (release 04-08-2014 CrysAlis171 .NET)
(compiled Aug  4 2014,14:34:23)
;
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXS (Sheldrick, 2008)'
_diffrn_ambient_environment      air
_diffrn_ambient_temperature      298.6(3)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 16.1183
_diffrn_detector_type            Eos
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.966
_diffrn_measurement_details
;
  1 omega -109.00   58.00   1.0000   17.6950
omega____ theta____ kappa____ phi______ frames
    -      -27.2013   19.0000   30.0000 167

  2 omega -110.00  -32.00   1.0000   17.6950
omega____ theta____ kappa____ phi______ frames
    -      -27.2013  -77.0000  -30.0000 78
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, Eos, Gemini ultra'
_diffrn_measurement_method       '\w scans'
_diffrn_orient_matrix_UB_11      -0.0893092000
_diffrn_orient_matrix_UB_12      -0.0978451000
_diffrn_orient_matrix_UB_13      0.0028538000
_diffrn_orient_matrix_UB_21      0.0237792000
_diffrn_orient_matrix_UB_22      -0.0292256000
_diffrn_orient_matrix_UB_23      -0.0332307000
_diffrn_orient_matrix_UB_31      0.0571090000
_diffrn_orient_matrix_UB_32      -0.0372359000
_diffrn_orient_matrix_UB_33      0.0184898000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0357
_diffrn_reflns_av_unetI/netI     0.0198
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.966
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            3202
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.966
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         28.180
_diffrn_reflns_theta_min         2.192
_diffrn_source                   'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    27.066
_exptl_absorpt_correction_T_max  0.039
_exptl_absorpt_correction_T_min  0.008
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.34i (release 04-08-2014 CrysAlis171 .NET)
(compiled Aug  4 2014,14:34:23)
Analytical numeric absorption correction using a multifaceted crystal
			model based on expressions derived by R.C. Clark & J.S. Reid.
(Clark, R. C. & Reid, J. S. (1995). Acta Cryst. A51, 887-897)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            black
_exptl_crystal_colour_primary    black
_exptl_crystal_density_diffrn    4.460
_exptl_crystal_description       ribbon
_exptl_crystal_F_000             1064
_exptl_crystal_size_max          0.2595
_exptl_crystal_size_mid          0.2451
_exptl_crystal_size_min          0.1889
_refine_diff_density_max         0.988
_refine_diff_density_min         -1.822
_refine_diff_density_rms         0.255
_refine_ls_extinction_coef       0.0020(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.172
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     20
_refine_ls_number_reflns         460
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.172
_refine_ls_R_factor_all          0.0573
_refine_ls_R_factor_gt           0.0445
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0922P)^2^+0.6949P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1502
_refine_ls_wR_factor_ref         0.1637
_reflns_Friedel_coverage         0.000
_reflns_number_gt                361
_reflns_number_total             460
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c7tc04798c2.cif
_cod_data_source_block           fw_cs3fe2br9_abs
_cod_original_cell_volume        915.7(2)
_cod_database_code               7236991
_shelx_shelxl_version_number     2014/7
_chemical_oxdiff_formula         'Cs3 Fe2 Br9'
_reflns_odcompleteness_completeness 99.78
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     26.32
_olex2_refinement_description
;
;
_olex2_submission_special_instructions 'No special instructions were received'